LMucko/crystallography-open-database huggingface dataset:
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 265 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013863
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 265 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.06
_cell_angle_gamma                90
_cell_length_a                   9.5267
_cell_length_b                   8.5688
_cell_length_c                   5.2553
_cell_formula_units_Z            4
_cell_volume                     402.977
_database_code_amcsd             0007309
_diffrn_ambient_temperature      265
_exptl_crystal_density_diffrn    3.772
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013863
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 280 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013864
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 280 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.15
_cell_angle_gamma                90
_cell_length_a                   9.5405
_cell_length_b                   8.5630
_cell_length_c                   5.2669
_cell_formula_units_Z            4
_cell_volume                     403.945
_database_code_amcsd             0007310
_diffrn_ambient_temperature      280
_exptl_crystal_density_diffrn    3.763
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013864
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 303 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013865
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 303 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.248
_cell_angle_gamma                90
_cell_length_a                   9.5613
_cell_length_b                   8.5691
_cell_length_c                   5.2668
_cell_formula_units_Z            4
_cell_volume                     404.852
_database_code_amcsd             0007311
_diffrn_ambient_temperature      303
_exptl_crystal_density_diffrn    3.754
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013865
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 323 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013866
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 323 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.219
_cell_angle_gamma                90
_cell_length_a                   9.5614
_cell_length_b                   8.5698
_cell_length_c                   5.2677
_cell_formula_units_Z            4
_cell_volume                     405.034
_database_code_amcsd             0007312
_diffrn_ambient_temperature      323
_exptl_crystal_density_diffrn    3.753
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013866
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 343 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013867
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 343 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.223
_cell_angle_gamma                90
_cell_length_a                   9.5633
_cell_length_b                   8.5715
_cell_length_c                   5.2686
_cell_formula_units_Z            4
_cell_volume                     405.253
_database_code_amcsd             0007313
_diffrn_ambient_temperature      343
_exptl_crystal_density_diffrn    3.751
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013867
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 363 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013868
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 363 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.221
_cell_angle_gamma                90
_cell_length_a                   9.5646
_cell_length_b                   8.5738
_cell_length_c                   5.2684
_cell_formula_units_Z            4
_cell_volume                     405.407
_database_code_amcsd             0007314
_diffrn_ambient_temperature      363
_exptl_crystal_density_diffrn    3.749
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013868
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 383 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013869
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 383 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.219
_cell_angle_gamma                90
_cell_length_a                   9.5666
_cell_length_b                   8.5753
_cell_length_c                   5.2691
_cell_formula_units_Z            4
_cell_volume                     405.622
_database_code_amcsd             0007315
_diffrn_ambient_temperature      383
_exptl_crystal_density_diffrn    3.747
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013869
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 423 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013870
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 423 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.218
_cell_angle_gamma                90
_cell_length_a                   9.5721
_cell_length_b                   8.5791
_cell_length_c                   5.2708
_cell_formula_units_Z            4
_cell_volume                     406.169
_database_code_amcsd             0007316
_diffrn_ambient_temperature      423
_exptl_crystal_density_diffrn    3.742
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013870
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 473 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013871
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 473 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.196
_cell_angle_gamma                90
_cell_length_a                   9.5762
_cell_length_b                   8.5728
_cell_length_c                   5.2715
_cell_formula_units_Z            4
_cell_volume                     406.155
_database_code_amcsd             0007317
_diffrn_ambient_temperature      473
_exptl_crystal_density_diffrn    3.742
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013871
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 573 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013872
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 573 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.173
_cell_angle_gamma                90
_cell_length_a                   9.5859
_cell_length_b                   8.5911
_cell_length_c                   5.2731
_cell_formula_units_Z            4
_cell_volume                     407.619
_database_code_amcsd             0007318
_diffrn_ambient_temperature      573
_exptl_crystal_density_diffrn    3.729
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013872
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 673 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013873
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 673 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.169
_cell_angle_gamma                90
_cell_length_a                   9.5942
_cell_length_b                   8.6018
_cell_length_c                   5.2752
_cell_formula_units_Z            4
_cell_volume                     408.653
_database_code_amcsd             0007319
_diffrn_ambient_temperature      673
_exptl_crystal_density_diffrn    3.719
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013873
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 773 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013874
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 773 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.130
_cell_angle_gamma                90
_cell_length_a                   9.5997
_cell_length_b                   8.6121
_cell_length_c                   5.2763
_cell_formula_units_Z            4
_cell_volume                     409.564
_database_code_amcsd             0007320
_diffrn_ambient_temperature      773
_exptl_crystal_density_diffrn    3.711
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013874
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 873 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013875
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 873 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.119
_cell_angle_gamma                90
_cell_length_a                   9.6080
_cell_length_b                   8.6219
_cell_length_c                   5.2778
_cell_formula_units_Z            4
_cell_volume                     410.530
_database_code_amcsd             0007321
_diffrn_ambient_temperature      873
_exptl_crystal_density_diffrn    3.702
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013875
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 973 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013876
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 973 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.118
_cell_angle_gamma                90
_cell_length_a                   9.6173
_cell_length_b                   8.6313
_cell_length_c                   5.2804
_cell_formula_units_Z            4
_cell_volume                     411.581
_database_code_amcsd             0007322
_diffrn_ambient_temperature      973
_exptl_crystal_density_diffrn    3.693
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013876
_amcsd_formula_title             LiGaSi2O6
Spontaneous strain variations through the low-temperature displacive phase transition of LiGaSi2O6 clinopyroxene Note: T = 1073 K
Camara, F.; Nestola, F.; Angel, R. J.; Ohashi, H.; European Journal of Mineralogy 21 (2009) 599–614; doi:10.1127/0935-1221/2009/0021-1926

data_9013877
_publ_section_title
;
 Spontaneous strain variations through the low-temperature displacive
 phase transition of LiGaSi2O6 clinopyroxene
 Note: T = 1073 K
;
_journal_name_full               'European Journal of Mineralogy'
_journal_page_first              599
_journal_page_last               614
_journal_paper_doi               10.1127/0935-1221/2009/0021-1926
_journal_volume                  21
_journal_year                    2009
_chemical_compound_source        Synthetic
_chemical_formula_structural     LiGa(Si2O6)
_chemical_formula_sum            'Ga Li O6 Si2'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 110.098
_cell_angle_gamma                90
_cell_length_a                   9.6260
_cell_length_b                   8.6433
_cell_length_c                   5.2813
_cell_formula_units_Z            4
_cell_volume                     412.649
_database_code_amcsd             0007323
_diffrn_ambient_temperature      1073
_exptl_crystal_density_diffrn    3.683
_cod_original_formula_sum        'Li Ga Si2 O6'
_cod_database_code               9013877
_amcsd_formula_title             LiGaSi2O6